{'fraction_non_alphanumeric': 0.03759315178546694, 'fraction_numerical': 0.03543230739396626, 'mean_word_length': 4.559525643000154, 'pattern_counts': {'":': 0, '<': 12, '<?xml version=': 0, '>': 14, 'https://': 0, 'lorem ipsum': 0, 'www.': 1, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 7, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Photoreactive Coating Material as an Effective and Durable Antimicrobial Composite in Reducing Bacterial Load on Surfaces in Livestock

Titanium dioxide (TiO2) is a well-known photocatalytic compound that can be used to effectively reduce the presence of pathogens in human and animal hospitals via ROS release. The aim of this study was to investigate the efficacy of a polymer-based composite layer containing TiO2 and zinc oxide (ZnO) against Escherichia coli (E. coli) of animal origin. We showed that the photocatalyst coating caused a significant (p < 0.001) reduction in pathogen numbers compared to the control with an average reduction of 94% over 30 min. We used six light sources of different wattages (4 W, 7 W, 9 W, 12 W, 18 W, 36 W) at six distances (35 cm, 100 cm, 150 cm, 200 cm, 250 cm, 300 cm). Samples (n = 2160) were taken in the 36 settings and showed no significant difference in efficacy between light intensity and distance. We also investigated the influence of organic contaminant that resulted in lower activity as well as the effect of a water jet and a high-pressure device on the antibacterial activity. We found that the latter completely removed the coating from the surface, which significantly (p < 0.0001) reduced its antibacterial potential. As a conclusion, light intensity and distance does not reduce the efficacy of the polymer, but the presence of organic contaminants does.


Introduction
Numerous research studies have investigated the potential of photocatalytic materials [1,2] for the purpose of creating self-cleaning surfaces [3], such as textiles [4] or antibacterial surfaces [5][6][7]. Other opportunities for application are to make implants safer [8], treat sewer [9], and reduce the odor caused by gas emission of livestock [10]. As a photocatalyst, TiO 2 needs UV-light to activate, however, it would be highly beneficial if activation could occur in the visible wavelength, requiring modification of the material's electrochemical properties. Toward this end, Asahi et al. found TiO 2 doped with nitrogen to be the most effective, as it changed the bandwidth of the activation wavelength of TiO 2 such that activation occurred at 500 nm, the range of visible light wavelength [11]. Tahmasebizad et al. described activation of TiO 2 doped with copper and nitrogen shifting to the visible light range [12]. Tallósy et al., in 2014, found that nano silver similarly impacted the activation of TiO 2 [13], and in a study from 2015, supported the importance of semiconductor nanoparticles [14]. Tobaldi et al., during their investigations, described the activation of nanostructure TiO 2 and silver particles photochromism to visible light [15]. Magalhães et al. established that doping with graphene shifted the activating wavelength range [16]. Finally, in the case of TiO 2 doped with copper in aerosol form, Alotaibi et al. described higher photocatalytic activity [17]. On the other hand, preserving nanomaterial plained by photo excited ZnO nanoparticles permeating across the cell wall and reacting with protein and carbohydrate molecules in the cytoplasm to inactivate them. In addition, release of ROS molecules also contributes to inactivation [41]. In favor of profoundly understanding the photocatalytic bactericide activity of TiO 2 , Takao et al. focused on the peptidoglycan layer of bacterial cell wall during their study. In the course of this investigation, results showed that the presence of peptidoglycan layer increases the bactericide effect of photocatalysis [42]. Rodríguez-González et al., in their review, also described lesions in the bacterial cell wall caused by ROS molecules and metal particles [34].
The aim of our studies was to demonstrate the efficacy of TiO 2 as a potential alternative to fight antimicrobial resistance, which has significant bacterial reduction capacity against environmental pathogens.

Materials and Methods
The aqueous photoreactive coating material used in this study consisted of TiO 2 (Degussa P25) and ZnO (Molar Chemicals) photocatalysts, while the surface immobilization of the particles was ensured by poly(ethyl acrylate-co-methyl methacrylate) (p(EA-co-MMA)) polymer [13].
Photocatalyst paint was applied to the surface with a brush in the afternoon of the day before the test days. The reference bacterial strain used in the tests was ATCC E. coli (LGC ATCC-25922, FDA strain Seattle 1946 (DSM 1103, NCIB 12210), Teddington, UK). We chose this bacterium because several studies have shown a link between contamination of food, especially poultry, with E. coli strains and human infection [43][44][45][46][47]. Furthermore, this bacteria is commonly used-not because of the disease it can cause-but because it is much easier to cultivate and handle in laboratories because of its low biological safety level (Class I). In most cases, the mediating role of poultry is associated with a higher risk than that of pork or beef [48][49][50]. E. coli strains that cause diarrhea of porcine origin have been shown to be able to transmit genes encoding Shiga toxin production with human Stx2 phage [51], and cattle are a major reservoir of Shiga toxin-producing E. coli strains [52]. To prepare the E. coli stock solution, E. coli stored at −80 • C was added to 400 mL of tryptone soy broth (TSB) and incubated at 37 • C for 18-24 h in a thermostat. A 150 mL suspension/surface/test volume of the stock solution was applied to both photocatalyst composite treated and untreated surfaces.
Preliminary tests have shown that it is worth sampling the wall surface for at least 480 min (8 h), during which time the control bacterial count is not significantly decreased. Sampling times were as follows: 00 min before E. coli application, 0 min after E. coli application, then 15, 30, 60, 90, 120, 240, 360, and 480 min. Sampling was performed with a COPAN (Copan Italia Spa, Brescia, Italy) sterile sampling stick. Samples were grafted onto Petri dishes containing tryptone-soy agar (90 mm × 14.2 mm, beam sterilized, without cams, Biolab Zrt., Budapest). A total of 2400 samples were taken over a period of one month using 36 different combinations of light intensity and spacing. Samples were placed in a 37 • C thermostat and Colony Forming Unit (CFU) counts were performed after 18-24 h incubation time. Samples with >1000 CFU were counted as 1000 CFU for graphical representation, as were samples with >300 CFU; samples with <300 CFU were counted exactly. The standard deviations were calculated in Excel using the following formula: ; where x is the mean value of the average (number1, number2, ...) and n is the sample size.
A single light source was placed in the room, and then the designated surface was illuminated from the specified distance for 8 h. For the test, six different wattages of light sources with the same emission spectra (see later) were used: 4 W (320 lux/m 2 ), 7 W (600 lux/m 2 ), 9 W (806 lux/m 2 ), 12 W (1521 lux/m 2 ), 18 W (2000 lux/m 2 ) and 36 W (3960 lux/m 2 ). The wattages of the light sources were converted into lumen per m 2 (lux/m 2 ), the unit of luminous flux. The conversion was performed using the formula Φ V (lm) = P (W) × η (lm/W), where P is the wattage and luminous efficacy (η) is taken to be 90 lm/W. The choice of distances was based on the fact that light sources in stables are on average 2.5-3 m above the animal contact surfaces. On this basis, we selected six different distances, the smallest being 35 cm, followed by 100 cm, 150 cm, 200 cm, 250 cm and 300 cm.
The light intensity (expressed as W/m 2 ) on the irradiated surface of the photoreactive nanohybrid films was measured with a power meter (Thorlabs GmbH, Bergkirchen, Germany). During the measurement, the distance of the light sources from the surface was systematically increased and the corresponding light intensity values were measured. Thus, we determined how light intensity changes with increasing distance from the light source.
When examining the effect of organic pollutants, a layer of E. coli suspension from the stock solution was applied. After the bacterial suspension dried, a medium thick layer of pig feces was applied. This process was carried out with care to ensure uniform layer thickness. The parameters most similar to industrial conditions were the primary criteria for selection of the settings, and therefore the two lowest wattage lamps (4 W and 7 W) were selected at the highest distance (300 cm).
The purpose of the mechanical impact test was to check the adherence of the dispersion paint on the wall surface after cleaning impacts. The coating was applied to the designated area on the wall in the afternoon of the day before the test to provide sufficient drying time. In one of the tests, a water jet wash was applied the following morning. The hose was connected to a tap in the room and the surface was washed using normal tap water pressure, no other cleaning equipment or chemicals were used. As a second part of the mechanical impact test, another prepared wall surface was washed with a high-pressure cleaning device on the wall part treated with the designated paint. After washing, and after the wall surfaces had dried, E. coli suspension was applied to the surfaces.
In both cases, tap water was used for washing. Washing by both methods was carried out at the same distance from the surface. The mechanical contact time was approximately 15-20 s for both the water jet and high-pressure cleaning. The effect of water jet washing was tested with a 7 W LED lamp at a distance of 300 cm and the effect of high-pressure washing was tested with a 4 W lamp at a distance of 300 cm.
The results were evaluated using the random forest method due to the large number of variables. Random forest is a machine learning method that generates many different decision trees. For numerical variables, the results are averaged, for categorical variables the algorithm counts which result is the most frequent. The decision trees are always generated using only a random subset of variables, so averaging the results of the different decision trees gives a more accurate result than generating a decision tree using all the variables. Information about the importance of the variables is also obtained, which is calculated by the algorithm by looking at the extent to which the hit rates of the decision trees decrease when the variable is omitted. The more the hit rate decreases with the omission of a variable, the more important that variable is.
The hit rate indicates the proportion of data that the model has classified into the correct category. The p-values for the variables were determined using the CART (Classification and Regression Tree) method (random forest), in which the algorithm generates a decision tree based on the variables. The analysis was performed using the R program version 4.0.5 (R Foundation for Statistical Computing, Vienna, Austria), and the packages ggplot2, partykit and strucchange.

Results of the Luminance and Distance Test
The detailed chemical characterization of the photocatalyst particles containing the composite layer used in this study was presented in our previous papers. Briefly, we reported several times that this transparent polyacrylate with good film-forming properties is highly applicable for the surface immobilization of semiconductor photocatalyst particles. At ideal composition (i.e., at optimal photocatalyst/polymer ratio) the polymer component provides appropriate mechanical stability for the composite layer [13,53] while the free photocatalyst particle surfaces are able to exert the photocatalytic properties [54]. Moreover, it was also presented that at higher photocatalyst loading the polymer coverage is not complete and accessible photocatalyst particles can be found on the surface of composite layers and the bacteria obviously preferred the high energy photocatalyst surfaces of the composite layer instead of the low energy polymer [55].
The emission spectra of the light sources used during the experiments can be seen on Figure S1. Each LED lamp has a similar spectrum and emits only in the visible light range. However, Figure S2 shows that the measured light intensity values were systematically changed with the increased wattage and it was inversely proportional to the square of the distance from the source. At lowest distance (35 cm) the light intensity of the 4 W LED was only 14.8 W/m 2 , while the intensity of the strongest LED lamp (36 W) was much higher (106 W/m 2 ). At larger distances (250-300 cm), however, very low intensity values were measured (<0.5 W/m 2 ) in each case.
In the first setting, the 4 W light source test, the photocatalyst composite treated section showed a significant decrease in CFU count on average from the 15th min onwards, until reaching only 2.3% of the baseline count after 30 min. After 90 min, at least 99.5% of the bacteria was eliminated by the photoreactive polymer. On the non-treated surface, there was a confluent increase in CFU counts ( Figure 1).

Results of the Luminance and Distance Test
The detailed chemical characterization of the photocatalyst particles containing composite layer used in this study was presented in our previous papers. Briefly, we ported several times that this transparent polyacrylate with good film-forming prope is highly applicable for the surface immobilization of semiconductor photocatalyst p cles. At ideal composition (i.e., at optimal photocatalyst/polymer ratio) the polymer c ponent provides appropriate mechanical stability for the composite layer [13,53] while free photocatalyst particle surfaces are able to exert the photocatalytic properties Moreover, it was also presented that at higher photocatalyst loading the polymer cove is not complete and accessible photocatalyst particles can be found on the surface of c posite layers and the bacteria obviously preferred the high energy photocatalyst surf of the composite layer instead of the low energy polymer [55].
The emission spectra of the light sources used during the experiments can be see Figure S1. Each LED lamp has a similar spectrum and emits only in the visible light ra However, Figure S2 shows that the measured light intensity values were systematic changed with the increased wattage and it was inversely proportional to the square o distance from the source. At lowest distance (35 cm) the light intensity of the 4 W L was only 14.8 W/m 2 , while the intensity of the strongest LED lamp (36 W) was m higher (106 W/m 2 ). At larger distances (250-300 cm), however, very low intensity va were measured (<0.5 W/m 2 ) in each case.
In the first setting, the 4 W light source test, the photocatalyst composite treated tion showed a significant decrease in CFU count on average from the 15th min onwa until reaching only 2.3% of the baseline count after 30 min. After 90 min, at least 99.5 the bacteria was eliminated by the photoreactive polymer. On the non-treated surf there was a confluent increase in CFU counts ( Figure 1). As shown in the statistical analysis, power wattage did not affect overall efficacy. After 15 min, the 36W LED lamp reduced the amount of E. coli by the greatest amount at a distance of 250 cm. resulting in 99.7% reduction after 60 min.

Results of Organic Pollutant Effect
Before the application of organic contamination and E. coli, no colonies were detected on the photocatalyst-treated surface, whereas 127 (4 W) and 1000 (7 W) CFU were counted on the control surface. Samples taken immediately after application of bacterial suspension and pig manure all had >1000 CFU. All samples taken from non-treated surfaces retained >1000 CFU counts.
Samples taken from the dye-treated area with a 4 W LED lamp after 15 min did not show a significant CFU reduction, however, by 30 min the composite layer showed 78.8% efficiency. From that point on, the amount of CFUs that could be counted steadily decreased, from 89 at minute 60, to 45 at minute 90, and 40 at minute 480. Thus, the photocatalyst layer coated with pig manure illuminated from 300 cm with a 4 W lamp killed 96% of the bacteria overall. When using the 7 W lamp, 205 CFU were counted at 30 min, so 79.5% of the bacteria was killed. At 120 min 112 CFUs were recorded and at 480 min 54 CFUs. Thus, at a distance of 300 cm, when using the 7 W LED lamp, the coating showed an overall efficiency of 94.6% (Figure 2).

Results of Organic Pollutant Effect
Before the application of organic contamination and E. coli, no colonies were detec on the photocatalyst-treated surface, whereas 127 (4 W) and 1000 (7 W) CFU were coun on the control surface. Samples taken immediately after application of bacterial susp sion and pig manure all had >1000 CFU. All samples taken from non-treated surfaces tained >1000 CFU counts.
Samples taken from the dye-treated area with a 4 W LED lamp after 15 min did show a significant CFU reduction, however, by 30 min the composite layer showed 78 efficiency. From that point on, the amount of CFUs that could be counted steadily creased, from 89 at minute 60, to 45 at minute 90, and 40 at minute 480. Thus, the pho catalyst layer coated with pig manure illuminated from 300 cm with a 4 W lamp ki 96% of the bacteria overall. When using the 7 W lamp, 205 CFU were counted at 30 m so 79.5% of the bacteria was killed. At 120 min 112 CFUs were recorded and at 480 min CFUs. Thus, at a distance of 300 cm, when using the 7 W LED lamp, the coating show an overall efficiency of 94.6% (Figure 2).

Results of the Mechanical Impact Test
When testing the water-washed surface prior to E. coli smearing, 300 CFU counted for the control samples and no colonies were grown for the treated samples. A the bacterial suspension was smeared, >1000 CFU was found on samples taken from b parts. This number did not change at subsequent time points in the control area, and >1 CFU was still observed at the 480th minute. For the dye-treated area, only 300 CFU counted at minute 15, which further decreased to 1 CFU at minute 30. This value maintained until the 120th minute, but no CFUs were found on the sample taken at 240th minute. From this point on, at minutes 240, 360 and 480, there were also no CF i.e., E. coli was completely eliminated (100%) from the surface tested.
After washing with the high-pressure equipment, low CFU values were obtained fore the bacterial suspension was applied, 1 CFU for the control and 2 CFU for the coa treated one. After application of E. coli, >1000 CFU was observed on all samples. On untreated control surface, this value was maintained up to 480 min. However, there

Results of the Mechanical Impact Test
When testing the water-washed surface prior to E. coli smearing, 300 CFU was counted for the control samples and no colonies were grown for the treated samples. After the bacterial suspension was smeared, >1000 CFU was found on samples taken from both parts. This number did not change at subsequent time points in the control area, and >1000 CFU was still observed at the 480th minute. For the dye-treated area, only 300 CFU was counted at minute 15, which further decreased to 1 CFU at minute 30. This value was maintained until the 120th minute, but no CFUs were found on the sample taken at the 240th minute. From this point on, at minutes 240, 360 and 480, there were also no CFUs, i.e., E. coli was completely eliminated (100%) from the surface tested.
After washing with the high-pressure equipment, low CFU values were obtained before the bacterial suspension was applied, 1 CFU for the control and 2 CFU for the coating treated one. After application of E. coli, >1000 CFU was observed on all samples. On the untreated control surface, this value was maintained up to 480 min. However, there was no decrease in CFU in the samples taken from the treated surface, with >1000 CFU in the samples taken at the 480th minute ( Figure 3).
Biomedicines 2022, 10, x FOR PEER REVIEW 7 no decrease in CFU in the samples taken from the treated surface, with >1000 CFU in samples taken at the 480th minute ( Figure 3).

Figure 3.
Washing test on the treated and untreated surfaces from a distance of 300 cm. In the of normal water jet washing, the paint-treated area had only 300 CFU at minute 15, which fu decreased to 1 CFU by minute 30, and by minute 120, the bacterial count reduction was 100%. A washing with high pressure equipment, there was no CFU reduction in samples taken from treated surface even after 480 min.

Statistical Analysis
Our aim was to determine the effectiveness of the photoreactive coating treated face in reducing bacterial counts. For the treated and untreated wall surfaces teste parallel, 3 × 3 samples were taken before (00) and 0, 15, 30, 60, 90, 120, 240, 360 and min after the coating was applied. During the experiment, the wall was illuminate different distances (35 cm, 100 cm, 150 cm, 200 cm, 250 cm and 300 cm) with diffe wattages of light sources (4 W, 7 W, 9 W, 12 W, 18 W, 37 W). For the first branching o random forest method, the p-value of all variables was less than 0.001 for luminous in sity and distance, but overall, the effects of watt, distance and time were more mode on the model hit rate compared to the treatment (Figure 4).
When examining the importance of the variables (treatment, distance, wattage, time), treatment was found to have the highest value (3.3416). The other variables significantly lower values: watt (0.5265), distance (0.2328), and finally time (0.1638). also confirms the effectiveness of the treatment, as no effect will be observed if the tr ment is abandoned.   . Washing test on the treated and untreated surfaces from a distance of 300 cm. In the case of normal water jet washing, the paint-treated area had only 300 CFU at minute 15, which further decreased to 1 CFU by minute 30, and by minute 120, the bacterial count reduction was 100%. After washing with high pressure equipment, there was no CFU reduction in samples taken from the treated surface even after 480 min.

Statistical Analysis
Our aim was to determine the effectiveness of the photoreactive coating treated surface in reducing bacterial counts. For the treated and untreated wall surfaces tested in parallel, 3 × 3 samples were taken before (00) and 0, 15, 30, 60, 90, 120, 240, 360 and 480 min after the coating was applied. During the experiment, the wall was illuminated at different distances (35 cm, 100 cm, 150 cm, 200 cm, 250 cm and 300 cm) with different wattages of light sources (4 W, 7 W, 9 W, 12 W, 18 W, 37 W). For the first branching of the random forest method, the p-value of all variables was less than 0.001 for luminous intensity and distance, but overall, the effects of watt, distance and time were more moderate on the model hit rate compared to the treatment (Figure 4).
When examining the importance of the variables (treatment, distance, wattage, and time), treatment was found to have the highest value (3.3416). The other variables had significantly lower values: watt (0.5265), distance (0.2328), and finally time (0.1638). This also confirms the effectiveness of the treatment, as no effect will be observed if the treatment is abandoned.
In the statistical analysis, we compared the results obtained after the organic pollutant was applied with the results of the luminosity-distance experiment obtained in our first study. We analyzed the values using the random forest method described earlier, where we used only the experimental results of our first study at 4 W and 7 W at a distance of 300 cm. The resulting CFU values were divided into groups for easier statistical analysis and then examined to see what factors influence which category the given bacterial count falls into. The group numbers we chose always indicate the lowest value (e.g., 50 indicates values of 50 or more but less than 100). Except for treatment (p < 0.0001), the effect of the variables in the experiment was negligible. Regarding the importance of the variables (treatment, organic pollutant, time, and wattage), treatment was again the most important (6.6135), with negligible effects of organic pollutant (0.7262), time (0.4894), and wattage (0.2927). Again, if the treatment is omitted, no effective reduction in bacterial counts can be expected.  Comparison of control and treated surfaces by random forest method as a function of light intensity and illumination distance. When examining luminance and distance, the p-value of all variables was less than 0.001 at the first branching, but overall, the effects of wattage, distance, and time were more moderate on the model hit rate compared to the treatment.
In the statistical analysis, we compared the results obtained after the organic pollutant was applied with the results of the luminosity-distance experiment obtained in our first study. We analyzed the values using the random forest method described earlier, where we used only the experimental results of our first study at 4 W and 7 W at a distance of 300 cm. The resulting CFU values were divided into groups for easier statistical analysis Comparison of control and treated surfaces by random forest method as a function of light intensity and illumination distance. When examining luminance and distance, the p-value of all variables was less than 0.001 at the first branching, but overall, the effects of wattage, distance, and time were more moderate on the model hit rate compared to the treatment.
In the third experiment, we first compared high-pressure and water-jet washing, and then compared the results after mechanical treatment with the results without mechanical treatment. The difference between water jet and high-pressure cleaning is significant (p < 0.0001), as is the difference in watts (p < 0.0001), with the effect of time being negligible. Compared to the control, the results show that high-pressure washing has a significant effect on bacterial counts (p < 0.0001), while the effect of normal water jet is negligible (p = 0.9998). Among the variables, treatment is also the most important (5.1756), but the effect of the mechanical action itself is significant (3.2573), while the effects of wattage (0.6328) and time (0.1387) are negligible.

Discussion
The photocatalytic activation of the polymer based composite layer containing TiO 2 and ZnO particles tested proved to be effective-as also described by Tallósy and Tobaldi [13,15]-our results showed a significant difference between control and treated surfaces (p < 0.001), with treatment being the most important statistical variable in each study.
The photocatalytic material was mixed with a polymeric binder, but it was not blocked by the binder, in contrast to the studies of Leng et al. [56]. The efficacy of the binder-free compound was also demonstrated under hospital conditions [57].
It was ascertained that in laboratory circumstances TiO 2 possessed a bactericide effect. After 30 min treatment in crude water and UV overshine, E. coli and S. aureus were inactivated at 92.6% and 94.2%. Photocatalytic sterilization potential was effective after 24 h of the beginning of lighting [58]. Nakano et al. investigated multi resistant Pseudomonas aeruginosa-t (P. aeruginosa) in addition to E. coli and S. aureus after TiO 2 treatment, and noticed that Gram-positive bacteria was inactivated at high efficiency, but Gram-negatives required more [59]. Ibrahim et al. demonstrated bactericide activity of TiO 2 at a rate of 97% against E.coli and 95% against S. aureus [60]. Previously, Mohl et al. revealed that TiO 2 has excellent antimicrobial activity against methicillin-susceptible S. aureus (MSSA) and methicillin-resistant S. aureus (MRSA) [61]. Shimizu et al. detected effective deactivation of E.coli with use of composites by carbon nanotubes and TiO 2 [62]. Janus et al. described that adding TiO 2 in concrete at 10% by weight has significant antibacterial effect against E. coli, it was even able to completely destroy the bacteria [63]. For 5% TiO 2 : Cu multifunctional thin films, Alotaibi et al. formulated that it was successfully able to eliminate antibacterial activity contra E. coli and S. aureus. Furthermore, researchers showed that photocatalytic efficiency increased greatly because of interstitial and substitutional Cu [17]. Liao et al. described in their review that Cu 2 O/TiO 2 inactivated 100% of E. coli after 60 min [64]. Usage of TiO 2 coating as an opportunity is confirmed by further research [65,66]. In a Listeria monocytogenes biofilm, the number of bacteria decreased 3 log/CFU after 90 min treatment with TiO 2 and UV-A light [67]. Bartomeuf et al. examined a photoactive layer, which showed increased efficiency to 400 nm threshold against L. monocytogenes. In addition, the number of bacteria decreased significantly after 20 min UV-A lighting [68].
Our research has shown that the combination of light source wattages (4 W, 7 W, 9 W, 12 W, 18 W and 36 W) we tested, placed at different distances (35 cm, 100 cm, 150 cm, 200 cm, 250 cm, 300 cm), did not show a significant difference in the efficiency of the photocatalyst layer (p < 0.001). This can be explained by the bacteria's defense mechanisms against ROS compounds circulating in the eye during photocatalysis [69]. No other comparative study of this kind has been published. In their studies, Rizzo et al. described the ability of TiO 2 -containing polymer to completely eliminate E. coli bacteria in 10 min for a 250 W light source [70], a result that suggests a much better efficiency in time compared to our studies, but we did not perform 10 min sampling. The difference was probably caused by the different TiO 2 compound and concentration, and the efficiency was not tested on a surface but in liquid (wastewater). This suggests that it would be worthwhile to investigate the effect of higher wattage light sources and to sample at shorter time intervals for CFU calculation.
The antibacterial effect of ZnO nanoparticles was also investigated against E. coli, with use of dispersion-containing and not containing ZnO particles. Dispersion which contained nanoparticles represented powerful antibacterial activity proportional to the concentration of ZnO, and bacteriostatic effect was noticed in 12 mmol/L concentration [71]. Later, the antibacterial effect of ZnO was confirmed by Sirelkhatim et al. [72], and Lallo da Silva et al., and described more powerful photocatalytic activity and biocompatibility compare to TiO 2 [73]. The antibacterial effect of a nanocomposite made by TiO 2 and ZnO particles was investigated by Chakra et al. against E. coli and S. aureus bacteria. Apart from the pronounced antibacterial action, results revealed that TiO 2 and ZnO particles worked in synergism [74]. Happy et al. made spherical shaped, 60-80 nm sized ZnO nanoparticles with green synthesis and investigated its antibacterial activity. The ZnO compound showed dose-dependent antibacterial effect against E. coli (IC 50 value was 20 µg/mL) [75]. Naseer et al. investigated the antibacterial potential of ZnO nanoparticles made by plant based green synthesis against E. coli and S. aureus bacteria. In the case of S. aureus, standard antibiotics achieved inhibition zone with a range of 4-13 mm, while the ZnO nano compound range was 14-37 mm [76]. The TiO 2 nanoparticles synthesized by eco-friendly plant extract impacted anti-biofilm effect against Staphylococcus epidermidis and P. aeruginosa bacteria [77]. Important to note is that excessive usage of nanoparticles increases output to the environment, which may be harmful to the ecosystem. In swine gut whose feed contained ZnO, Ciesinksi et al. found multi resistant E. coli bacteria 28.9-30.2% compared to 5.8-14% in the control group. Unfortunately, this refers to the resistant strains [78].
In terms of efficacy against E. coli, we found that a significant reduction in CFU counts was observed from the 15th minute onwards, with an average reduction of 97% in CFU counts at 30 min, 98% at 60 min, 99% at 120 min and 99.9% at 480 min compared to the initial CFU counts. Baek et al., however, when testing ZnO, found a reduction of only 72% after 6 h of illumination [79], while Wu et al. in TiO 2 tests described bacterial count reductions of 20% after 5 min, 90% after 30 min and 100% after 90 min-but TiO 2 was modified with palladium [39]. Chen et al. found eradication of 92.6% in 30 min in unrefined water and 100% in the same time in isosmotic water [58]. However, Ibrahim et al. observed only a 16% reduction in bacterial counts after 30 min, 67% after 90 min, 80% after 120 min and 97% after 180 min [60]. In comparison, we observed a faster and more effective antibacterial effect, with an average of 97% in 30 min. Janus et al. experienced 100% eradication in as little as 60 min [63], and Liao et al. experienced the same [64]. In contrast, Dong et al. described 100% eradication after 24 h of treatment [80]. Nakano et al., using TiO 2 on a glass slide, described a reduction of the initial bacterial count of 1.5 × 10 5 CFU/mL to 1.5 × 10 4 after 2 h, 1.5 × 10 3 after 4 h and 1 × 10 2 after 8 h [59]. In contrast, Alotaibi et al. found a decrease in bacterial counts from an initial 1 × 10 8 CFU/mL to 1.5 × 10 5 in 2 h and 1 × 10 3 in 4 h for copper doped TiO 2 [17]. However, it should be pointed out that in our studies different concentrations and brightness were used. Based on the published results, it can be concluded that light intensity and distance indeed do not have a significant effect on the photocatalytic antibacterial efficacy of TiO 2 . Our results and those of previous studies are compared in Table 1.  [60] In our organic pollutant study, pig manure reduced the efficiency, but this was not significant (p < 0.001). Similar experiences were reported by Chen et al. who investigated the inactivation of E. coli by TiO 2 in unrefined and isosmotic water [58], however, they did not investigate surface contamination. However, Rizzo et al. conducted their study with wastewater, in which E. coli bacteria was fully eradicated in 10 min under 250 W illumination and in only 60 min under sunlight illumination [70]. However, no previous study has been described to investigate the effect of contamination of a surface with photocatalyst containing organic fertilizer. It can be concluded that the photocatalyst containing polymer is able to retain its antibacterial activity, but more time is needed for the effect to develop.
The results of the mechanical penetration experiments show that the water jet has little effect, while the high-pressure device completely removed the layer from the wall. Regarding the stability of the photocatalytic compound, Mori et al. described that it is advisable to fix the photocatalyst to a substrate so that it is not damaged by the reactions that occur [1]. It follows from our studies that the treated surfaces can be cleaned with a mild application, but that the strong applications, also used in disinfection, completely remove the photocatalyst layer, and therefore its reapplication is necessary.

Conclusions
Overall, it can be concluded that the antibacterial activity of the photocatalyst does not depend on either distance or light intensity. When contaminated with organic matter, the effectiveness is slightly reduced, but the difference is only in the length of time required. Washing with water jets is resistant to the coating, but high-pressure treatments remove it. Bacteria can develop several defense mechanisms against light-induced ROS compounds, which may explain the lack of difference in efficacy between different light intensities. Other bacteria of public health importance (Staphylococcus aureus, Pseudomonas aeruginosa) and fungi (Aspergillus spp., Candida spp.) should be tested in the future.
Supplementary Materials: The following supporting information can be downloaded at: https: //www.mdpi.com/article/10.3390/biomedicines10092312/s1, Figure S1: The emission spectra of LED light sources with increasing wattage.; Figure S2: The measured light intensity values of LED light sources as a function of the distance.